Post on 05-Mar-2015
Embed Size (px)
www.rsc.org/dalton | Dalton Transactions
Synthesis of inorganic nanomaterialsC. N. R. Rao,*a,b S. R. C. Vivekchand,a Kanishka Biswasa,b and A. Govindaraja,bReceived 1st June 2007, Accepted 9th July 2007 First published as an Advance Article on the web 6th August 2007 DOI: 10.1039/b708342d Synthesis forms a vital aspect of the science of nanomaterials. In this context, chemical methods have proved to be more effective and versatile than physical methods and have therefore, been employed widely to synthesize a variety of nanomaterials, including zero-dimensional nanocrystals, one-dimensional nanowires and nanotubes as well as two-dimensional nanolms and nanowalls. Chemical synthesis of inorganic nanomaterials has been pursued vigorously in the last few years and in this article we provide a perspective on the present status of the subject. The article includes a discussion of nanocrystals and nanowires of metals, oxides, chalcogenides and pnictides. In addition, inorganic nanotubes and nanowalls have been reviewed. Some aspects of coreshell particles, oriented attachment and the use of liquidliquid interfaces are also presented.
Nanoscience involves a study of materials where at least one of the dimensions is in the 1100 nm range. Properties of such materials are strongly dependant on their size and shape. Nanomaterials include zero-dimensional nanocrystals, one-dimensional nanowires and nanotubes and two-dimensional nanolms and nanowalls. Synthesis forms an essential component of nanoscience and nanotechnology. While nanomaterials have been generated by physical methods such as laser ablation, arc-discharge and evaporation, chemical methods have proved to be more effective, as they provide better control as well as enable different sizes, shapes and functionalization. Chemical synthesis of nanomaterials has been reviewed by a few authors,16 but innumerable improvements and better methods are being reported continually in the last few years. In accomplishing the synthesis and manipulation of the nanomaterials, a variety of reagents and strategies have been employed besides a wide spectrum of reaction conditions. In view of the intense research activity related to nanomaterials synthesis, we have prepared this perspective to present recent developments and new directions in this area. In doing so, we have dealt with all classes of inorganic nanomaterials. In writing such an article, it has been difcult to do justice to the vast number of valuable contributions which have appeared in the literature in last the two to three years. We had to be necessarily succinct and restrict ourselves mainly to highlighting recent results.
in the case of metal nanocrystals. Metal oxide nanocrystals are generally prepared by the decomposition of precursor compounds such as metal acetates, acetylacetonates and cupferronates in appropriate solvents, often under solvothermal conditions. Metal chalcogenide or pnictide nanocrystals are obtained by the reaction of metal salts with a chalcogen or pnicogen source or the decomposition of single source precursors under solvothermal or thermolysis conditions. Addition of suitable capping agents such as long-chain alkane thiols, alkyl amines and trioctylphosphine oxide (TOPO) during the synthesis of nanocrystals enables the control of size and shape. Monodisperse nanocrystals are obtained by post-synthesis size-selective precipitation.
2.1 Metals Reduction of metal salts in the presence of suitable capping agents such as polyvinylpyrrolidone (PVP) is the common method to generate metal nanocrystals. Solvothermal and other reaction conditions are employed for the synthesis, to exercise control over their size and shape of the nanocrystals.1,2,7 Furthermore, the sealed reaction conditions and presence of organic reagents reduce the possibility of atmospheric oxidation of the nanocrystals. The popular citrate route to colloidal Au, rst described by Hauser and Lynn,8 involves the addition of chloroauric acid to a boiling solution of sodium citrate.9 The average diameter of the nanocrystals can be varied over the 10100 nm range by varying the concentration of reactants. Au nanocrystals with diameters between 1 and 2 nm are obtained by the reduction of HAuCl4 with tetrakis(hydroxymethyl)phosphonium chloride (THPC) which also acts as a capping agent.10 Following the early work of Brust and co-workers,11 the general practice employed to obtain organic-capped metal nanocrystals is to use a bi-phasic mixture of an organic solvent and the aqueous solution of the metal salt in the presence of a phase-transfer reagent. The metal ion is transferred across the organicwater interface by the phase transfer reagent and subsequently reduced to yield sols of metal nanocrystals. Metal nanocrystals in the aqueous phase can also be transferred to a nonaqueous medium by using alkane thiols to obtain organosols.12,13 This method has been used to thiolize This journal is The Royal Society of Chemistry 2007
Nanocrystals are zero-dimensional particles and can be prepared by several chemical methods, typical of them being reduction of salts, solvothermal synthesis and the decomposition of molecular precursors, of which the rst is the most common method useda Chemistry and Physics of Materials Unit, DST unit on nanoscience and CSIR Centre of Excellence in Chemistry, Jawaharlal Nehru Centre for Advanced Scientic Research, Jakkur P. O., Bangalore, 560064, India. E-mail: email@example.com; Fax: +91 80 22082760 b Solid State and Structural Chemistry Unit, Indian Institute of Science, Bangalore, 560012, India
3728 | Dalton Trans., 2007, 37283749
C. N. R. Rao obtained his PhD degree from Purdue University and DSc degree from the University of Mysore. He is the Linus Pauling Research Professor at the Jawaharlal Nehru Centre for Advanced Scientic Research and Honorary Professor at the Indian Institute of Science (both at Bangalore). His research interests are in the chemistry of materials. He has authored nearly 1000 research papers and edited or written 30 books in materials chemistry. A member of several academies including the Royal Society and the US National Academy of Sciences, he is the recipient of the Einstein Gold Medal of UNESCO, Hughes Medal of the Royal Society, and the Somiya Award of the International Union of Materials Research Societies (IUMRS). In 2005, he received the Dan David Prize for materials research from Israel and the rst India Science Prize. S. R. C. Vivekchand received his BSc degree from The American College, Madurai in 2001. He is a student of the integrated PhD programme of Jawaharlal Nehru Centre for Advanced Scientic Research, Bangalore and received his MS degree in 2004. He has worked primarily on material chemistry aspects of one-dimensional nanomaterials. Kanishka Biswas received his BSc degree from Jadavpur University, Kolkata in 2003. He is a student of the integrated PhD programme of Indian Institute of Science, Bangalore and received his MS degree in 2006. He has worked primarily on the synthesis and characterization of inorganic nanomaterials. A. Govindaraj obtained his PhD degree from University of Mysore and is a Senior Scientic Ofcer at the Indian Institute of Science, and Honorary Faculty Fellow at the Jawaharlal Nehru Centre for Advanced Scientic Research. He works on different types of nanomaterials. He has authored more than 100 research papers and co-authored a book on nanotubes and nanowires.
C. N. R. Rao
S. R. C. Vivekchand
Pd nanocrystals with magic numbers of atoms.14,15 A method to produce gold nanocrystals free from surfactants would be to reduce HAuCl4 by sodium napthalenide in diglyme.16 Liz-Mar an and co-workers17 have prepared nanoscale Ag z nanocrystals by using dimethylformamide as both a stabilizing agent and a capping agent. By using tetrabutylammonium borohydride or its mixture with hydrazine, Jana and Peng18 obtained monodisperse nanocrystals of Au, Cu, Ag, and Pt. In this method, AuCl3 , Ag(CH3 COO), Cu(CH3 COO)2 , and PtCl4 were dispersed in toluene with the aid of long-chain quaternary ammonium salts and reduced with tetrabutylammonium borohydride which is toluene-soluble. The reaction can be scaled up to produce gram quantities of nanocrystals. Mirkin and co-workers1921 have devised two synthetic routes for nanoprisms of Ag. In the rst method, Ag nanoprisms (Fig. 1a) are produced by irradiating a mixture of sodium citrate and bis(p-sulfonatophenyl) phenylphosphine dihydrate dipotassium capped Ag nanocrystals with a uorescent lamp. In the second method, AgNO3 is reduced with a mixture of borohydride and hydrogen peroxide.21 The latter method has been extended to synthesize branched nanocrystals of Au of the type shown in Fig. 1b and 1c.22,23 The shape and colour of Au nanoparticles can be altered by NAD(P)H-mediated growth in the presence of ascorbic acid.24 This journal is The Royal Society of Chemistry 2007
The method yields dipods, tripods and tetrapods (nanocrystals with 2, 3 and 4 arms respectively, the one with 4 arms generally being tetrahedral). Icosahedral Au nanocrystals are obtained by the reaction of HAuCl4 with PVP in aqueous media.25 Rightbipyramid (75150 nm in edge length) nanocrystals of Ag (Fig. 2) have been prepared by the addition of NaBr during the polyol reduction of AgNO3 in the presence of PVP.26 Cu nanoparticles of pyramidal shape have been made by an electrochemical procedure.27 Nanoparticles of Rh and Ir have been prepared by the reduction of the appropriate compounds in the ionic liquid, 1-n-butyl3-methylimidazoliumhexauorophosphate, in the presence of hydrogen.28 Synthesis and functionalization of gold nanoparticles in ionic liquids is also reported, wherein the colour of the gold nanoparticles can be tuned by ch